#------------------------------------------------------------------------------
#$Date: 2016-03-25 14:32:06 +0200 (Fri, 25 Mar 2016) $
#$Revision: 179900 $
#$URL: svn://www.crystallography.net/cod/cif/7/01/96/7019671.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7019671
loop_
_publ_author_name
'Zheng, Yun-Yun'
'Wen, Ru'
'Kong, Xiang-Jian'
'Long, La-Sheng'
'Huang, Rong-Bin'
'Zheng, Lan-Sun'
_publ_section_title
;
 Assembly of an undeca-nuclear nickel substituted POM through
 polycarboxylate ligand.
;
_journal_issue                   33
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              9871
_journal_page_last               9875
_journal_paper_doi               10.1039/c2dt12507b
_journal_volume                  41
_journal_year                    2012
_chemical_formula_sum            'C24 H103 N15 Ni12 O99 P2 W18'
_chemical_formula_weight         6261.97
_chemical_name_systematic
;
?
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 105.63(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   38.794(8)
_cell_length_b                   20.940(4)
_cell_length_c                   17.201(3)
_cell_measurement_reflns_used    8498
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      26.00
_cell_measurement_theta_min      3.09
_cell_volume                     13456(5)
_computing_cell_refinement       PROCESS-AUTO
_computing_data_collection       'PROCESS-AUTO (Rigaku Corporation, 1998)'
_computing_data_reduction
'teXsan (Molecular Structure Corporation, Rigaku Corporation, 1999)'
_computing_molecular_graphics    'SHELXTL V.5.0 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Rigaku R-AXIS RAPID Imaging Plate'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.2083
_diffrn_reflns_av_sigmaI/netI    0.1690
_diffrn_reflns_limit_h_max       47
_diffrn_reflns_limit_h_min       -47
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            57640
_diffrn_reflns_theta_full        26.00
_diffrn_reflns_theta_max         26.00
_diffrn_reflns_theta_min         3.09
_exptl_absorpt_coefficient_mu    17.071
_exptl_absorpt_correction_T_max  0.505
_exptl_absorpt_correction_T_min  0.148
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   '(ABSCOR; Higashi, 1995)'
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    3.091
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             11368
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.04
_platon_squeeze_details
;
SQUEEZE removed 2 disordered (H2en)2+ and
7 disordered water molecules per formula unit. This valueis
calculated based upon elemental analysis data and the squeeze void count electrons.
;
_refine_diff_density_max         4.677
_refine_diff_density_min         -2.758
_refine_diff_density_rms         0.476
_refine_ls_extinction_coef       0.000094(13)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.033
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     743
_refine_ls_number_reflns         13580
_refine_ls_number_restraints     42
_refine_ls_restrained_S_all      1.032
_refine_ls_R_factor_all          0.1194
_refine_ls_R_factor_gt           0.0885
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1193P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2325
_refine_ls_wR_factor_ref         0.2516
_reflns_number_gt                8498
_reflns_number_total             13580
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2dt12507b.txt
_cod_data_source_block           compound_1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_cell_volume        13457(5)
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               7019671
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
W3 W 0.26404(3) 0.08223(4) 0.00934(5) 0.0521(3) Uani 1 1 d .
W6 W 0.18449(3) 0.08774(4) 0.39253(5) 0.0500(3) Uani 1 1 d .
W2 W 0.33338(3) 0.17056(4) 0.15990(5) 0.0498(3) Uani 1 1 d .
W1 W 0.39667(3) 0.08826(4) 0.30131(5) 0.0498(3) Uani 1 1 d .
W5 W 0.32972(5) 0.0000 -0.04994(7) 0.0601(4) Uani 1 2 d S
W4 W 0.39948(3) 0.08904(4) 0.10268(6) 0.0584(3) Uani 1 1 d .
W8 W 0.03294(3) 0.08164(4) 0.16098(5) 0.0526(3) Uani 1 1 d .
W7 W 0.11149(3) 0.16878(4) 0.28374(5) 0.0524(3) Uani 1 1 d .
W9 W 0.10666(3) 0.08847(5) 0.45557(5) 0.0603(3) Uani 1 1 d .
W10 W 0.02731(4) 0.0000 0.33277(8) 0.0590(4) Uani 1 2 d S
Ni3 Ni 0.24681(11) 0.0000 0.17867(17) 0.0412(9) Uani 1 2 d S
Ni5 Ni 0.16240(8) 0.07299(11) 0.17882(14) 0.0450(7) Uani 1 1 d .
Ni7 Ni 0.09393(12) 0.0000 0.0764(2) 0.0488(10) Uani 1 2 d S
Ni2 Ni 0.30586(8) 0.07623(11) 0.30817(14) 0.0427(7) Uani 1 1 d .
Ni4 Ni 0.24662(8) 0.14690(11) 0.18468(13) 0.0445(7) Uani 1 1 d .
Ni6 Ni 0.10140(9) 0.14893(12) 0.07724(15) 0.0524(8) Uani 1 1 d .
O49 O 0.1150(6) 0.0000 0.4787(9) 0.049(5) Uani 1 2 d S
O30 O 0.2413(5) 0.0000 -0.0286(10) 0.044(4) Uani 1 2 d SU
O48 O 0.0608(4) 0.0585(6) 0.3938(8) 0.054(4) Uani 1 1 d .
O18 O 0.0645(4) 0.0757(6) 0.1010(8) 0.042(3) Uani 1 1 d .
O15 O 0.2477(4) 0.0729(6) 0.1018(8) 0.052(4) Uani 1 1 d .
O10 O 0.1928(6) 0.0000 0.1526(9) 0.052(6) Uani 1 2 d S
H10A H 0.1858 0.0000 0.0934 0.063 Uiso 1 2 calc SR
O39 O 0.1558(5) 0.0947(8) 0.4738(8) 0.067(5) Uani 1 1 d .
O26 O 0.3248(4) 0.2528(7) 0.1491(8) 0.056(4) Uani 1 1 d .
O17 O 0.1265(4) 0.1401(5) 0.1992(7) 0.052(4) Uani 1 1 d .
O25 O 0.3696(4) 0.1605(6) 0.1035(7) 0.050(4) Uani 1 1 d .
O46 O 0.0113(6) 0.0000 0.1173(11) 0.053(6) Uani 1 2 d S
O23 O 0.4233(5) 0.0992(7) 0.2180(9) 0.063(5) Uani 1 1 d .
O5 O 0.1915(4) 0.1463(6) 0.1445(7) 0.047(4) Uani 1 1 d .
O4 O 0.2467(4) 0.2094(6) 0.2788(7) 0.044(4) Uani 1 1 d .
O14 O 0.3038(4) 0.1422(5) 0.2171(7) 0.043(3) Uani 1 1 d .
O42 O 0.0992(4) 0.1634(7) 0.3895(7) 0.056(4) Uani 1 1 d .
O47 O 0.0992(5) 0.1202(8) 0.5413(9) 0.073(5) Uani 1 1 d .
O29 O 0.2937(5) 0.0651(6) -0.0652(8) 0.057(4) Uani 1 1 d .
O8 O 0.2528(4) 0.0701(6) 0.2578(7) 0.040(3) Uani 1 1 d .
H8A H 0.2377 0.0684 0.2951 0.048 Uiso 1 1 calc R
O24 O 0.3019(4) 0.1400(6) 0.0617(8) 0.055(4) Uani 1 1 d .
Ni1 Ni 0.36080(12) 0.0000 0.4372(2) 0.0475(10) Uani 1 2 d S
Ni8 Ni 0.23670(19) 0.0000 -0.3130(2) 0.092(2) Uani 1 2 d S
O12 O 0.1265(5) 0.0000 0.2056(9) 0.038(4) Uani 1 2 d S
O22 O 0.3537(4) 0.0594(6) 0.1759(7) 0.040(3) Uani 1 1 d .
O11 O 0.3071(7) 0.0000 0.2161(10) 0.056(6) Uani 1 2 d S
O9 O 0.1274(5) 0.0705(6) 0.0659(8) 0.056(4) Uani 1 1 d .
H9A H 0.1378 0.0682 0.0200 0.067 Uiso 1 1 calc R
O38 O 0.2259(4) 0.1189(7) 0.4468(8) 0.056(4) Uani 1 1 d .
O45 O 0.0006(4) 0.1349(6) 0.1068(8) 0.058(4) Uani 1 1 d .
O44 O 0.0692(6) 0.0000 0.2464(10) 0.049(5) Uani 1 2 d S
O21 O 0.3742(4) 0.1669(6) 0.2581(8) 0.050(4) Uani 1 1 d .
O28 O 0.3076(5) 0.0000 0.0744(9) 0.040(5) Uani 1 2 d S
O2 O 0.3591(5) 0.0731(6) 0.5180(7) 0.053(4) Uani 1 1 d .
O37 O 0.1225(4) 0.0572(6) 0.3291(6) 0.049(4) Uani 1 1 d .
O41 O 0.0636(4) 0.1355(6) 0.2352(8) 0.061(4) Uani 1 1 d .
O33 O 0.4317(6) 0.1168(8) 0.0553(11) 0.083(6) Uani 1 1 d .
O36 O 0.1869(6) 0.0000 0.4203(10) 0.049(5) Uani 1 2 d S
O16 O 0.1893(4) 0.0721(5) 0.2955(7) 0.037(3) Uani 1 1 d .
O27 O 0.2322(5) 0.1333(7) -0.0495(7) 0.062(5) Uani 1 1 d .
O13 O 0.3613(4) 0.0676(6) 0.3461(8) 0.050(4) Uani 1 1 d .
O20 O 0.4297(4) 0.1151(6) 0.3833(9) 0.055(4) Uani 1 1 d .
O32 O 0.4120(7) 0.0000 0.1152(13) 0.063(7) Uani 1 2 d S
O31 O 0.3637(5) 0.0609(6) 0.0096(8) 0.059(4) Uani 1 1 d .
O19 O 0.4124(7) 0.0000 0.3016(11) 0.065(7) Uani 1 2 d S
O7 O 0.3095(6) 0.0000 0.3833(10) 0.056(6) Uani 1 2 d S
H7A H 0.2933 0.0000 0.4184 0.067 Uiso 1 2 calc SR
N2 N 0.2405(5) 0.2321(8) 0.1179(9) 0.052(5) Uani 1 1 d .
H2C H 0.2560 0.2326 0.0866 0.062 Uiso 1 1 calc R
O35 O 0.1592(5) 0.1681(7) 0.3533(8) 0.060(4) Uani 1 1 d .
O5W O 0.0629(7) 0.0000 -0.0425(13) 0.067(6) Uani 1 2 d SU
O40 O 0.1064(5) 0.2476(7) 0.2689(10) 0.069(5) Uani 1 1 d .
O50 O -0.0070(8) 0.0000 0.3809(13) 0.077(8) Uani 1 2 d S
N6 N 0.0716(6) 0.2298(8) 0.0845(11) 0.063(6) Uani 1 1 d .
H6C H 0.0584 0.2234 0.1194 0.076 Uiso 1 1 calc R
H6D H 0.0862 0.2633 0.1017 0.076 Uiso 1 1 calc R
P1 P 0.3299(2) 0.0000 0.1613(4) 0.0406(18) Uani 1 2 d S
P2 P 0.1114(2) 0.0000 0.2747(4) 0.0413(18) Uani 1 2 d S
O34 O 0.3380(9) 0.0000 -0.1400(13) 0.082(9) Uani 1 2 d S
O3 O 0.2507(6) 0.3116(7) 0.3112(9) 0.084(6) Uani 1 1 d .
N4 N 0.3056(6) 0.1434(8) 0.3944(9) 0.061(6) Uani 1 1 d .
H4C H 0.2833 0.1592 0.3857 0.073 Uiso 1 1 calc R
H4D H 0.3114 0.1245 0.4432 0.073 Uiso 1 1 calc R
N3 N 0.3349(6) 0.2287(9) 0.5453(11) 0.072(6) Uani 1 1 d .
H3C H 0.3331 0.2631 0.5744 0.108 Uiso 1 1 calc R
H3D H 0.3568 0.2122 0.5631 0.108 Uiso 1 1 calc R
H3E H 0.3188 0.1998 0.5500 0.108 Uiso 1 1 calc R
O1 O 0.3937(5) 0.1440(7) 0.5947(10) 0.080(6) Uani 1 1 d .
C8 C 0.3305(6) 0.1961(9) 0.3947(12) 0.050(5) Uani 1 1 d .
H8F H 0.3249 0.2156 0.3416 0.060 Uiso 1 1 calc R
H8G H 0.3547 0.1795 0.4066 0.060 Uiso 1 1 calc R
N1 N 0.4186(8) 0.0000 0.5044(13) 0.052(7) Uani 1 2 d S
H1A H 0.4317 0.0000 0.4676 0.062 Uiso 1 2 calc SR
C4 C 0.2480(6) 0.2654(9) 0.2596(11) 0.045(5) Uani 1 1 d U
C3 C 0.2467(6) 0.2887(9) 0.1713(12) 0.048(5) Uani 1 1 d U
H3F H 0.2275 0.3195 0.1527 0.058 Uiso 1 1 calc R
H3G H 0.2691 0.3090 0.1710 0.058 Uiso 1 1 calc R
C2 C 0.3904(8) 0.0934(11) 0.5525(14) 0.063(8) Uani 1 1 d .
C1 C 0.4250(9) 0.0631(11) 0.5494(15) 0.077(9) Uani 1 1 d .
H1F H 0.4398 0.0559 0.6039 0.092 Uiso 1 1 calc R
H1G H 0.4378 0.0918 0.5227 0.092 Uiso 1 1 calc R
C6 C 0.1775(7) 0.1915(9) 0.0951(10) 0.051(6) Uani 1 1 d .
C7 C 0.3284(7) 0.2473(10) 0.4583(11) 0.061(7) Uani 1 1 d .
H7F H 0.3454 0.2806 0.4557 0.073 Uiso 1 1 calc R
H7G H 0.3048 0.2663 0.4414 0.073 Uiso 1 1 calc R
O43 O 0.0113(5) 0.0617(7) 0.2527(9) 0.080(6) Uani 1 1 d .
O6 O 0.1451(5) 0.2033(7) 0.0712(8) 0.062(5) Uani 1 1 d .
N5 N 0.0796(6) 0.1613(8) -0.0429(10) 0.071(7) Uani 1 1 d .
H5C H 0.0958 0.1543 -0.0707 0.085 Uiso 1 1 calc R
H5D H 0.0608 0.1351 -0.0615 0.085 Uiso 1 1 calc R
O4W O 0.2073(10) 0.0000 -0.220(2) 0.115(11) Uani 1 2 d SU
C5 C 0.2036(7) 0.2331(11) 0.0665(14) 0.063(6) Uani 1 1 d U
H5F H 0.2038 0.2194 0.0127 0.075 Uiso 1 1 calc R
H5G H 0.1950 0.2767 0.0625 0.075 Uiso 1 1 calc R
O1W O 0.2693(9) 0.0712(8) -0.2506(14) 0.168(16) Uani 1 1 d .
O3W O 0.2535(16) 0.0000 -0.4175(16) 0.19(2) Uani 1 2 d S
C9 C 0.0681(9) 0.2296(12) -0.0486(16) 0.091(10) Uani 1 1 d .
H9F H 0.0891 0.2570 -0.0366 0.109 Uiso 1 1 calc R
H9G H 0.0541 0.2388 -0.1033 0.109 Uiso 1 1 calc R
C10 C 0.0485(7) 0.2421(12) 0.0034(14) 0.062(6) Uani 1 1 d U
H10F H 0.0275 0.2147 -0.0076 0.074 Uiso 1 1 calc R
H10G H 0.0406 0.2863 -0.0015 0.074 Uiso 1 1 calc R
O2W O 0.1959(9) 0.0737(15) -0.3577(17) 0.178(15) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O27 W3 O15 102.0(6) . .
O27 W3 O24 102.7(7) . .
O15 W3 O24 93.4(6) . .
O27 W3 O30 99.2(7) . .
O15 W3 O30 88.0(7) . .
O24 W3 O30 157.3(7) . .
O27 W3 O29 100.5(6) . .
O15 W3 O29 157.3(6) . .
O24 W3 O29 85.0(6) . .
O30 W3 O29 85.0(7) . .
O27 W3 O28 171.4(5) . .
O15 W3 O28 83.7(6) . .
O24 W3 O28 83.3(5) . .
O30 W3 O28 74.3(6) . .
O29 W3 O28 73.7(6) . .
O38 W6 O16 105.0(6) . .
O38 W6 O36 104.5(8) . .
O16 W6 O36 92.7(7) . .
O38 W6 O35 99.5(7) . .
O16 W6 O35 90.2(5) . .
O36 W6 O35 154.1(8) . .
O38 W6 O39 101.6(6) . .
O16 W6 O39 153.1(6) . .
O36 W6 O39 83.9(8) . .
O35 W6 O39 81.9(7) . .
O38 W6 O37 170.5(6) . .
O16 W6 O37 82.6(5) . .
O36 W6 O37 80.5(7) . .
O35 W6 O37 74.5(6) . .
O39 W6 O37 70.6(6) . .
O26 W2 O14 104.5(6) . .
O26 W2 O24 100.3(6) . .
O14 W2 O24 91.3(6) . .
O26 W2 O25 101.4(6) . .
O14 W2 O25 154.1(6) . .
O24 W2 O25 84.0(7) . .
O26 W2 O21 102.3(6) . .
O14 W2 O21 90.1(6) . .
O24 W2 O21 156.2(6) . .
O25 W2 O21 84.4(6) . .
O26 W2 O22 172.3(6) . .
O14 W2 O22 81.9(5) . .
O24 W2 O22 83.7(5) . .
O25 W2 O22 72.2(5) . .
O21 W2 O22 73.0(5) . .
O20 W1 O13 102.4(6) . .
O20 W1 O21 101.4(6) . .
O13 W1 O21 93.0(6) . .
O20 W1 O19 98.3(8) . .
O13 W1 O19 92.6(8) . .
O21 W1 O19 157.9(7) . .
O20 W1 O23 97.7(7) . .
O13 W1 O23 159.9(6) . .
O21 W1 O23 83.9(6) . .
O19 W1 O23 83.6(7) . .
O20 W1 O22 172.6(6) . .
O13 W1 O22 84.3(5) . .
O21 W1 O22 74.7(5) . .
O19 W1 O22 84.6(7) . .
O23 W1 O22 75.7(6) . .
O34 W5 O29 100.9(8) . 6
O34 W5 O29 100.9(8) . .
O29 W5 O29 90.5(9) 6 .
O34 W5 O31 102.7(9) . .
O29 W5 O31 156.2(6) 6 .
O29 W5 O31 88.4(7) . .
O34 W5 O31 102.7(9) . 6
O29 W5 O31 88.4(7) 6 6
O29 W5 O31 156.2(6) . 6
O31 W5 O31 83.3(9) . 6
O34 W5 O28 171.5(12) . .
O29 W5 O28 73.3(5) 6 .
O29 W5 O28 73.3(5) . .
O31 W5 O28 83.6(5) . .
O31 W5 O28 83.6(5) 6 .
O33 W4 O25 104.7(7) . .
O33 W4 O31 99.1(8) . .
O25 W4 O31 86.7(6) . .
O33 W4 O32 100.4(9) . .
O25 W4 O32 154.3(8) . .
O31 W4 O32 84.3(8) . .
O33 W4 O23 103.4(8) . .
O25 W4 O23 91.7(6) . .
O31 W4 O23 157.0(6) . .
O32 W4 O23 87.5(8) . .
O33 W4 O22 174.8(6) . .
O25 W4 O22 71.1(5) . .
O31 W4 O22 83.8(5) . .
O32 W4 O22 84.1(8) . .
O23 W4 O22 74.0(6) . .
O45 W8 O18 103.8(7) . .
O45 W8 O41 102.2(6) . .
O18 W8 O41 91.5(7) . .
O45 W8 O46 100.4(7) . .
O18 W8 O46 90.4(8) . .
O41 W8 O46 156.1(6) . .
O45 W8 O43 99.1(7) . .
O18 W8 O43 157.0(6) . .
O41 W8 O43 85.0(7) . .
O46 W8 O43 83.9(8) . .
O45 W8 O44 169.4(7) . .
O18 W8 O44 85.8(6) . .
O41 W8 O44 81.6(6) . .
O46 W8 O44 74.8(6) . .
O43 W8 O44 71.2(7) . .
O40 W7 O17 104.8(7) . .
O40 W7 O35 99.1(7) . .
O17 W7 O35 91.9(6) . .
O40 W7 O41 103.1(7) . .
O17 W7 O41 90.8(7) . .
O35 W7 O41 156.2(6) . .
O40 W7 O42 98.4(8) . .
O17 W7 O42 156.7(5) . .
O35 W7 O42 81.9(6) . .
O41 W7 O42 86.3(7) . .
O40 W7 O37 170.6(6) . .
O17 W7 O37 82.8(5) . .
O35 W7 O37 74.9(6) . .
O41 W7 O37 82.0(5) . .
O42 W7 O37 73.9(5) . .
O47 W9 O39 103.4(7) . .
O47 W9 O49 104.9(8) . .
O39 W9 O49 85.6(8) . .
O47 W9 O42 99.2(7) . .
O39 W9 O42 91.6(7) . .
O49 W9 O42 155.8(6) . .
O47 W9 O48 105.0(8) . .
O39 W9 O48 151.3(6) . .
O49 W9 O48 83.0(7) . .
O42 W9 O48 88.3(6) . .
O47 W9 O37 171.4(7) . .
O39 W9 O37 71.5(5) . .
O49 W9 O37 81.8(6) . .
O42 W9 O37 74.5(5) . .
O48 W9 O37 80.9(6) . .
O50 W10 O43 101.9(9) . 6
O50 W10 O43 101.9(9) . .
O43 W10 O43 87.5(10) 6 .
O50 W10 O48 103.6(8) . 6
O43 W10 O48 90.2(6) 6 6
O43 W10 O48 154.4(8) . 6
O50 W10 O48 103.6(8) . .
O43 W10 O48 154.4(8) 6 .
O43 W10 O48 90.2(6) . .
O48 W10 O48 81.1(8) 6 .
O50 W10 O44 171.9(9) . .
O43 W10 O44 72.5(7) 6 .
O43 W10 O44 72.5(7) . .
O48 W10 O44 82.5(6) 6 .
O48 W10 O44 82.5(6) . .
O8 Ni3 O8 96.1(6) . 6
O8 Ni3 O10 94.4(5) . .
O8 Ni3 O10 94.4(5) 6 .
O8 Ni3 O15 172.5(7) . 6
O8 Ni3 O15 82.6(5) 6 6
O10 Ni3 O15 93.1(6) . 6
O8 Ni3 O15 82.6(5) . .
O8 Ni3 O15 172.5(7) 6 .
O10 Ni3 O15 93.1(6) . .
O15 Ni3 O15 97.8(8) 6 .
O8 Ni3 O11 83.2(5) . .
O8 Ni3 O11 83.2(5) 6 .
O10 Ni3 O11 176.4(6) . .
O15 Ni3 O11 89.3(6) 6 .
O15 Ni3 O11 89.3(6) . .
O16 Ni5 O9 170.3(7) . .
O16 Ni5 O10 92.2(6) . .
O9 Ni5 O10 92.6(6) . .
O16 Ni5 O17 91.6(5) . .
O9 Ni5 O17 82.8(6) . .
O10 Ni5 O17 173.3(7) . .
O16 Ni5 O5 96.6(5) . .
O9 Ni5 O5 91.2(5) . .
O10 Ni5 O5 95.7(6) . .
O17 Ni5 O5 89.3(6) . .
O16 Ni5 O12 88.4(6) . .
O9 Ni5 O12 83.4(6) . .
O10 Ni5 O12 87.9(6) . .
O17 Ni5 O12 86.8(6) . .
O5 Ni5 O12 173.7(6) . .
O16 Ni5 Ni6 135.1(4) . .
O9 Ni5 Ni6 40.7(4) . .
O10 Ni5 Ni6 132.7(5) . .
O17 Ni5 Ni6 43.7(3) . .
O5 Ni5 Ni6 81.1(4) . .
O12 Ni5 Ni6 92.6(4) . .
O9 Ni7 O9 94.8(9) 6 .
O9 Ni7 O18 172.5(6) 6 .
O9 Ni7 O18 82.0(6) . .
O9 Ni7 O18 82.0(6) 6 6
O9 Ni7 O18 172.5(6) . 6
O18 Ni7 O18 100.4(8) . 6
O9 Ni7 O5W 97.4(6) 6 .
O9 Ni7 O5W 97.4(6) . .
O18 Ni7 O5W 89.8(6) . .
O18 Ni7 O5W 89.8(6) 6 .
O9 Ni7 O12 83.3(5) 6 .
O9 Ni7 O12 83.3(5) . .
O18 Ni7 O12 89.5(5) . .
O18 Ni7 O12 89.5(5) 6 .
O5W Ni7 O12 178.9(9) . .
O8 Ni2 O7 96.3(7) . .
O8 Ni2 N4 98.7(7) . .
O7 Ni2 N4 95.3(6) . .
O8 Ni2 O14 83.7(5) . .
O7 Ni2 O14 169.8(5) . .
N4 Ni2 O14 94.8(6) . .
O8 Ni2 O13 168.9(5) . .
O7 Ni2 O13 81.0(8) . .
N4 Ni2 O13 92.3(7) . .
O14 Ni2 O13 96.9(6) . .
O8 Ni2 O11 82.2(7) . .
O7 Ni2 O11 83.1(5) . .
N4 Ni2 O11 178.2(7) . .
O14 Ni2 O11 86.8(5) . .
O13 Ni2 O11 86.7(7) . .
O8 Ni4 O5 98.2(6) . .
O8 Ni4 O4 92.4(5) . .
O5 Ni4 O4 92.7(5) . .
O8 Ni4 N2 174.7(6) . .
O5 Ni4 N2 82.4(6) . .
O4 Ni4 N2 82.4(5) . .
O8 Ni4 O15 79.4(5) . .
O5 Ni4 O15 88.7(6) . .
O4 Ni4 O15 171.7(5) . .
N2 Ni4 O15 105.9(6) . .
O8 Ni4 O14 81.9(5) . .
O5 Ni4 O14 174.8(4) . .
O4 Ni4 O14 92.5(5) . .
N2 Ni4 O14 98.0(6) . .
O15 Ni4 O14 86.2(5) . .
O9 Ni6 N5 95.2(7) . .
O9 Ni6 O6 90.4(7) . .
N5 Ni6 O6 90.0(7) . .
O9 Ni6 O17 84.9(5) . .
N5 Ni6 O17 176.1(8) . .
O6 Ni6 O17 86.1(6) . .
O9 Ni6 N6 176.9(7) . .
N5 Ni6 N6 82.6(8) . .
O6 Ni6 N6 91.7(7) . .
O17 Ni6 N6 97.5(6) . .
O9 Ni6 O18 79.3(6) . .
N5 Ni6 O18 99.5(7) . .
O6 Ni6 O18 166.5(5) . .
O17 Ni6 O18 84.4(5) . .
N6 Ni6 O18 99.0(7) . .
O9 Ni6 Ni5 42.9(4) . .
N5 Ni6 Ni5 135.3(7) . .
O6 Ni6 Ni5 78.0(4) . .
O17 Ni6 Ni5 43.8(4) . .
N6 Ni6 Ni5 139.9(5) . .
O18 Ni6 Ni5 88.5(3) . .
W9 O49 W9 153.3(9) 6 .
W3 O30 W3 122.4(10) . 6
W10 O48 W9 156.8(8) . .
W8 O18 Ni7 131.9(7) . .
W8 O18 Ni6 129.1(7) . .
Ni7 O18 Ni6 94.2(6) . .
W3 O15 Ni3 134.5(7) . .
W3 O15 Ni4 124.7(7) . .
Ni3 O15 Ni4 96.0(6) . .
Ni3 O10 Ni5 125.0(6) . 6
Ni3 O10 Ni5 125.0(6) . .
Ni5 O10 Ni5 96.2(10) 6 .
W9 O39 W6 127.9(8) . .
W7 O17 Ni6 128.3(8) . .
W7 O17 Ni5 137.5(7) . .
Ni6 O17 Ni5 92.5(5) . .
W4 O25 W2 128.4(7) . .
W8 O46 W8 121.2(10) . 6
W4 O23 W1 121.3(9) . .
C6 O5 Ni4 115.5(15) . .
C6 O5 Ni5 124.4(15) . .
Ni4 O5 Ni5 120.1(6) . .
C4 O4 Ni4 112.6(12) . .
W2 O14 Ni2 137.0(8) . .
W2 O14 Ni4 127.7(6) . .
Ni2 O14 Ni4 93.1(5) . .
W9 O42 W7 123.4(7) . .
W5 O29 W3 124.8(6) . .
Ni3 O8 Ni2 105.2(6) . .
Ni3 O8 Ni4 101.0(5) . .
Ni2 O8 Ni4 98.8(6) . .
W2 O24 W3 148.1(8) . .
O7 Ni1 O2 96.0(6) . .
O7 Ni1 O2 96.0(6) . 6
O2 Ni1 O2 94.7(7) . 6
O7 Ni1 O13 81.9(6) . 6
O2 Ni1 O13 174.4(5) . 6
O2 Ni1 O13 90.6(5) 6 6
O7 Ni1 O13 81.9(6) . .
O2 Ni1 O13 90.6(5) . .
O2 Ni1 O13 174.4(5) 6 .
O13 Ni1 O13 83.9(7) 6 .
O7 Ni1 N1 177.2(8) . .
O2 Ni1 N1 82.1(6) . .
O2 Ni1 N1 82.1(6) 6 .
O13 Ni1 N1 100.1(6) 6 .
O13 Ni1 N1 100.1(6) . .
O1W Ni8 O1W 92.7(11) . 6
O1W Ni8 O3W 99.2(15) . .
O1W Ni8 O3W 99.2(15) 6 .
O1W Ni8 O2W 167.1(15) . 6
O1W Ni8 O2W 87.5(11) 6 6
O3W Ni8 O2W 93.5(14) . 6
O1W Ni8 O2W 87.5(11) . .
O1W Ni8 O2W 167.1(15) 6 .
O3W Ni8 O2W 93.5(14) . .
O2W Ni8 O2W 89.3(18) 6 .
O1W Ni8 O4W 89.3(12) . .
O1W Ni8 O4W 89.3(12) 6 .
O3W Ni8 O4W 167.6(18) . .
O2W Ni8 O4W 77.8(12) 6 .
O2W Ni8 O4W 77.8(12) . .
P2 O12 Ni5 125.8(6) . .
P2 O12 Ni5 125.8(6) . 6
Ni5 O12 Ni5 88.0(7) . 6
P2 O12 Ni7 124.5(12) . .
Ni5 O12 Ni7 90.7(5) . .
Ni5 O12 Ni7 90.7(5) 6 .
P1 O22 W1 126.1(7) . .
P1 O22 W2 126.2(8) . .
W1 O22 W2 89.3(4) . .
P1 O22 W4 126.6(7) . .
W1 O22 W4 88.6(5) . .
W2 O22 W4 87.7(4) . .
P1 O11 Ni3 125.4(11) . .
P1 O11 Ni2 125.8(9) . .
Ni3 O11 Ni2 89.1(7) . .
P1 O11 Ni2 125.8(9) . 6
Ni3 O11 Ni2 89.1(7) . 6
Ni2 O11 Ni2 90.0(6) . 6
Ni6 O9 Ni7 104.2(8) . .
Ni6 O9 Ni5 96.4(5) . .
Ni7 O9 Ni5 102.3(7) . .
P2 O44 W8 124.6(6) . 6
P2 O44 W8 124.6(6) . .
W8 O44 W8 89.1(7) 6 .
P2 O44 W10 127.5(10) . .
W8 O44 W10 89.8(6) 6 .
W8 O44 W10 89.8(6) . .
W1 O21 W2 122.6(7) . .
P1 O28 W3 126.1(6) . 6
P1 O28 W3 126.1(6) . .
W3 O28 W3 88.8(6) 6 .
P1 O28 W5 127.5(12) . .
W3 O28 W5 87.9(4) 6 .
W3 O28 W5 87.9(4) . .
C2 O2 Ni1 111.0(16) . .
P2 O37 W6 124.5(9) . .
P2 O37 W7 124.0(7) . .
W6 O37 W7 87.6(4) . .
P2 O37 W9 130.7(8) . .
W6 O37 W9 89.2(4) . .
W7 O37 W9 88.0(4) . .
W8 O41 W7 149.9(10) . .
W6 O36 W6 151.9(10) 6 .
W6 O16 Ni5 142.4(8) . .
W1 O13 Ni2 133.6(7) . .
W1 O13 Ni1 129.7(7) . .
Ni2 O13 Ni1 94.3(7) . .
W4 O32 W4 151.3(14) 6 .
W4 O31 W5 153.2(8) . .
W1 O19 W1 143.6(14) . 6
Ni1 O7 Ni2 100.9(8) . 6
Ni1 O7 Ni2 100.9(8) . .
Ni2 O7 Ni2 103.4(8) 6 .
C5 N2 C3 109.5(17) . .
C5 N2 Ni4 106.9(13) . .
C3 N2 Ni4 111.5(11) . .
W7 O35 W6 121.9(8) . .
C10 N6 Ni6 107.2(14) . .
O11 P1 O28 110.9(13) . .
O11 P1 O22 109.9(7) . 6
O28 P1 O22 108.7(6) . 6
O11 P1 O22 109.9(7) . .
O28 P1 O22 108.7(6) . .
O22 P1 O22 108.7(11) 6 .
O12 P2 O37 113.3(7) . 6
O12 P2 O37 113.3(7) . .
O37 P2 O37 104.9(10) 6 .
O12 P2 O44 111.0(10) . .
O37 P2 O44 106.9(8) 6 .
O37 P2 O44 106.9(8) . .
C8 N4 Ni2 112.8(14) . .
N4 C8 C7 111.3(18) . .
C1 N1 C1 121(2) . 6
C1 N1 Ni1 105.6(16) . .
C1 N1 Ni1 105.6(16) 6 .
O4 C4 O3 122.1(18) . .
O4 C4 C3 124.2(17) . .
O3 C4 C3 113.8(16) . .
N2 C3 C4 107.8(15) . .
O1 C2 O2 119(3) . .
O1 C2 C1 115(2) . .
O2 C2 C1 126(2) . .
C2 C1 N1 111(2) . .
O6 C6 O5 125(2) . .
O6 C6 C5 119.0(19) . .
O5 C6 C5 116(2) . .
N3 C7 C8 119.9(17) . .
W10 O43 W8 126.4(11) . .
C6 O6 Ni6 130.2(12) . .
C9 N5 Ni6 103.0(15) . .
N2 C5 C6 115.1(19) . .
C10 C9 N5 111(2) . .
C9 C10 N6 107(2) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W3 O27 1.739(14) .
W3 O15 1.874(15) .
W3 O24 1.928(14) .
W3 O30 1.965(9) .
W3 O29 1.973(16) .
W3 O28 2.461(13) .
W6 O38 1.750(16) .
W6 O16 1.760(12) .
W6 O36 1.894(4) .
W6 O35 1.973(16) .
W6 O39 2.013(14) .
W6 O37 2.442(14) .
W2 O26 1.755(14) .
W2 O14 1.801(13) .
W2 O24 1.909(14) .
W2 O25 1.924(13) .
W2 O21 1.981(14) .
W2 O22 2.449(12) .
W1 O20 1.725(15) .
W1 O13 1.798(17) .
W1 O21 1.917(13) .
W1 O19 1.946(8) .
W1 O23 1.993(15) .
W1 O22 2.420(12) .
W5 O34 1.66(2) .
W5 O29 1.919(16) 6
W5 O29 1.919(16) .
W5 O31 1.920(15) .
W5 O31 1.920(15) 6
W5 O28 2.509(17) .
W4 O33 1.764(18) .
W4 O25 1.894(15) .
W4 O31 1.908(16) .
W4 O32 1.924(6) .
W4 O23 1.962(15) .
W4 O22 2.515(14) .
W8 O45 1.748(13) .
W8 O18 1.805(15) .
W8 O41 1.871(13) .
W8 O46 1.962(9) .
W8 O43 2.020(19) .
W8 O44 2.438(14) .
W7 O40 1.673(15) .
W7 O17 1.809(13) .
W7 O35 1.914(16) .
W7 O41 1.948(15) .
W7 O42 2.004(13) .
W7 O37 2.465(14) .
W9 O47 1.712(15) .
W9 O39 1.852(18) .
W9 O49 1.904(4) .
W9 O42 1.914(14) .
W9 O48 1.914(15) .
W9 O37 2.502(12) .
W10 O50 1.75(3) .
W10 O43 1.868(14) 6
W10 O43 1.868(14) .
W10 O48 1.887(13) 6
W10 O48 1.887(13) .
W10 O44 2.48(2) .
Ni3 O8 1.972(12) .
Ni3 O8 1.972(12) 6
Ni3 O10 2.02(2) .
Ni3 O15 2.026(14) 6
Ni3 O15 2.026(14) .
Ni3 O11 2.25(3) .
Ni5 O16 1.996(11) .
Ni5 O9 2.049(14) .
Ni5 O10 2.054(16) .
Ni5 O17 2.073(14) .
Ni5 O5 2.082(14) .
Ni5 O12 2.199(15) .
Ni5 Ni6 2.992(4) .
Ni7 O9 2.006(16) 6
Ni7 O9 2.006(16) .
Ni7 O18 2.064(14) .
Ni7 O18 2.064(14) 6
Ni7 O5W 2.07(2) .
Ni7 O12 2.240(16) .
Ni2 O8 2.010(15) .
Ni2 O7 2.034(11) .
Ni2 N4 2.046(16) .
Ni2 O14 2.074(11) .
Ni2 O13 2.080(15) .
Ni2 O11 2.258(12) .
Ni4 O8 2.017(11) .
Ni4 O5 2.064(16) .
Ni4 O4 2.082(12) .
Ni4 N2 2.101(16) .
Ni4 O15 2.114(14) .
Ni4 O14 2.139(15) .
Ni6 O9 1.964(15) .
Ni6 N5 2.027(16) .
Ni6 O6 2.068(18) .
Ni6 O17 2.070(12) .
Ni6 N6 2.072(18) .
Ni6 O18 2.210(14) .
O49 W9 1.904(4) 6
O30 W3 1.965(9) 6
O10 Ni5 2.054(16) 6
O46 W8 1.962(9) 6
O5 C6 1.29(2) .
O4 C4 1.22(2) .
Ni1 O7 1.96(2) .
Ni1 O2 2.081(13) .
Ni1 O2 2.081(13) 6
Ni1 O13 2.116(14) 6
Ni1 O13 2.116(14) .
Ni1 N1 2.23(3) .
Ni8 O1W 2.060(19) .
Ni8 O1W 2.060(19) 6
Ni8 O3W 2.07(4) .
Ni8 O2W 2.20(3) 6
Ni8 O2W 2.20(3) .
Ni8 O4W 2.20(4) .
O12 P2 1.46(2) .
O12 Ni5 2.199(15) 6
O22 P1 1.532(14) .
O11 P1 1.46(2) .
O11 Ni2 2.258(12) 6
O44 P2 1.58(2) .
O44 W8 2.438(14) 6
O28 P1 1.512(16) .
O28 W3 2.461(13) 6
O2 C2 1.27(3) .
O37 P2 1.509(12) .
O36 W6 1.894(4) 6
O32 W4 1.924(6) 6
O19 W1 1.946(8) 6
O7 Ni2 2.034(11) 6
N2 C5 1.46(3) .
N2 C3 1.48(2) .
N6 C10 1.46(3) .
P1 O22 1.532(14) 6
P2 O37 1.509(12) 6
O3 C4 1.30(2) .
N4 C8 1.47(3) .
N3 C7 1.50(3) .
O1 C2 1.27(3) .
C8 C7 1.55(2) .
N1 C1 1.52(2) .
N1 C1 1.52(2) 6
C4 C3 1.58(3) .
C2 C1 1.50(4) .
C6 O6 1.24(3) .
C6 C5 1.52(3) .
N5 C9 1.49(3) .
C9 C10 1.35(4) .
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
1 0.000 0.438 -0.012 2083.0 148.5
2 0.500 -0.004 -0.006 2082.9 148.4
3 0.250 0.250 0.500 20.8 3.2
4 0.250 0.750 0.500 20.8 3.5
5 0.750 0.250 0.500 20.8 3.5
6 0.750 0.750 0.500 20.8 3.2
